Share this document with a friend

16

Transcript

XPS Study of Multilayer Multicomponent Films

Alexander V. Lubenchenkoa,∗, Alexander A. Batrakova, Alexey B. Pavolotskyb, Olga I. Lubenchenkoa,Dmitriy. A. Ivanova

aNational Research University MPEI, Krasnokazarmennaya, 14, Moscow 111250, RussiabChalmers University of Technology, Gteborg, 41296, Sweden

Abstract

In the paper, we propose XPS-based quantitative method for depth profile analysis of chemical and phasecomposition of multi-component and multi-layer samples. The method includes: (1) new method for back-ground subtraction accounting for depth non-uniformity of electron energy losses; (2) new method for photo-electron line decomposition into elementary peaks, which accounts for physical nature of the decompositionparameters; (3) joint solving of both background subtraction and photoelectron line decomposition problems;(4) criterion for assessing of line decomposition accuracy; (5) simple formula for layer thickness extractionfor multi-element and multi-layer sample. We apply the developed method for analysis of multilayer niobiumoxide and sub-oxide films before and in course of ion milling.

Keywords: XPS; Chemical and phase analysis; Depth profiling; XPS background subtracting; XPS linedecomposition; Niobium oxide

1. Introduction

X-ray Photoelectron Spectroscopy (XPS) is one ofthe most demanded methods of the surface analy-sis [1]. XPS allows extracting elemental and phasecomposition of the analyzed surfaces. For that, afterbackground subtraction, position of the peaks formedby inelastically and elastically scattered photoelec-trons in the XPS spectrum is determined. Intensitiesof those peaks are interpreted into the relative con-centrations of the elements. The standard methodfor interpretation of XPS data is based on the as-sumption about uniform distribution of the elementsacross the whole depth of analysis. In reality thoughsample surface is always nonuniform and can be rep-resented as consisting of layers. Failure to account

∗Corresponding authorEmail address: [email protected] (Alexander V.

Lubenchenko)

for that leads to significant errors. For example, as-sume a sample has on its surface a layer of thicknessd1 of material other than the the rest of the sam-ple. In such case, following the Bouguer law, inten-sity of the peaks formed by the photo electrons un-der that surface layer will be reduced by the factor ofexp (−d1/λ1), where λ1 is electron mean free path inthat surface layer. In case of XPS with Mg/Al-anodeX-ray source, electron mean free path is of the or-der of a few nanometers. Consequently, even as thinas 1 nm surface layer will noticeably misrepresent theconcentrations calculated by the standard mean con-centration method.

For analysis of multilayer samples, more sophisti-cated calculation approach is needed. In paper [2],relationships for elements’ relative concentrations ina layer were derived. However, for that one needsto assume the layer model and solve nonlinear sys-tem of equation for extracting of layer thicknesses.Analytic solution of such system of equations is pre-

Preprint submitted to Applied Surface Science January 25, 2017

*ManuscriptClick here to view linked References

sented in paper [3]. Using of the methods accountingfor multilayer surface structure, one needs though tofind each element’s partial peak intensity. This prob-lem in turn depends on the accurate solution of thefollowing standard problems of XPS: (1) Subtractionof background due to multiple inelastically scatteredphotoelectrons; (2) Line decomposition into partialpeaks of not scattered and elastically scattered pho-toelectrons. These problems are significantly inter-linked.

In this paper, we present a new method for solv-ing of the standard problems of XPS. This includesbackground subtraction accounting for inelastic scat-tering nonuniform by the depth, as well as line de-composition into partial peaks, which is based onthe physical model for photoelectron peak forming.These two problems are solved together within thepresented approach. Presented in this paper, accountfor sample nonuniformity by depth significantly in-creases analysis accuracy as compared with the stan-dard approach.

Sample surface usually not only is multilayer, buteach layer itself is multicomponent and often multi-phase. Layer-by-layer interpretation of such samples’XPS spectra is a complex reverse problem with multi-ple unknown parameters. For correct solving of sucha problem, we propose: (1) Method for backgroundsubtraction accounting for electron energy losses dif-ferent in volume and at surface; (2) Parameters forbackground and line shape calculation fixed for thewhole range of the spectrum; (3) Line shape param-eters calculated based on the Handbook of X-RayPhotoelectron Spectroscopy [4] spectra for pure uni-form surfaces; (4) Formulas for chemically bonded el-ements photoelectron inherent peak width; (5) Jointinterpretation of different lines of the element withinthe same model. We also propose a criterion forjudging the quality of line decomposition to choosebetween alternative solutions. We suggest that cal-culations of mean relative stoichiometric coefficientsshould give the same result, when based either ondifferent lines intensities, or on partial intensities ofthe peaks of the line together with chemical shift (see(14)).

We applied the presented method to analysis ofchemical and phase composition of niobium oxide

films. Interest to niobium thin films and its com-pounds is motivated by its superconducting proper-ties and consequent application in cryoelectronic de-vices. Surface oxide films affect negatively on super-conducting properties of niobium, particularly whenused as thin film. There are a number of papers, e.g.[5, 6, 7, 8, 9], dedicated to XPS analysis of Nb ox-ide films. However, there are no known publicationscommunicating results of XPS analysis of phase com-position of surface niobium oxide films. The presentpaper attempts to fill this gap.

2. Experimental Details

In this paper, we studied niobium surface oxidefilms before and after ion profiling. Niobium was de-posited on silicon substrate by magnetron sputteringof 99.95% Nb in Ar with the help of Pfeiffer VacuumSLS630G sputtering cluster tool. Thickness of sput-tered Nb was 200 nm. Immediately after unloadingthe samples from the deposition system, the sampleswere covered by oxidation protecting layer of spunphotoresist. Right before loading the samples to theXPS analysis chamber, the protecting layer was re-moved in an ultrasonic bath filled with acetone fol-lowed by iso-propanol. This way, the total exposuretime of the samples to atmospheric air was about 10minutes.

XPS spectra were recorded with the help ofNanofab 25 (NT-MDT) electron-ion spectroscopyplatform. The base pressure in the analysis chamberwas at the level of 10−8 Pa provided by a titaniumsublimation pump and an ion pump. The residualpressure and composition of vacuum were monitoredby a Bayard-Alpert vacuum gauge and a secondaryion mass-spectrometer. The load-lock was pumpedwith a turbo-molecular pump. In the load-lock, itwas possible to store a number of samples at theresidual pressure of 10−6 Pa. For XPS analysis, theX-ray source SPECS XR 50 with a dual Al/Mg anodewas used providing 1486.6 eV and 1253.6 eV photons.The X-ray source was located at 54.7 degrees relativeto the analyzer axis. For surface charge neutralizing,flood electron gun SPECS FG 15/40 was used.

Semispheric electrostatic energy analyzer SPECSPhoibos 225 allowed recording of spectra in a broad

2

range of energies between 0 and 15 keV in the an-gle range of ±15 degrees with an energy resolutionof 0.6 eV FWHM measured at 15 keV. Energy ana-lyzer was calibrated with a use of reference Cu, Agand Au samples. Energy resolution of spectrometerat Ag 3d5/2 line was found to be 0.78 eV for non-monochromatic Mg Kα. All survey spectra scanswere taken at a pass energy of 80 eV. The detailedscans of strong lines were in most cases recorded aswide as needed just to encompass the peak(s) of in-terest and were obtained with a pass energy of 20 eV.All spectra were recorded with use of Mg anode ofthe X-ray source. The energy analyzer was operatedin Fixed Analyzer Transmission (FAT) mode.

For cleaning and ion profiling of the samples, an ionsource SPECS IQE 12/38 was used. The ion sourcehad differential pumping and was fed with 99.9995%pure Ar. For ion profiling, the ion beam was scanningthe 2.8 × 4.0 mm2 area at the incidence angle of 50degrees to the surface normal. Ion profiling includedtotal 9 cycles of sputtering with recording of XPSspectra before sputtering and after each cycle. Forsputtering cycles #1 – #6, each cycle was 20 minutelong and beam energy and current were 0.5 keV and0.5µA, respectively. For sputtering cycles #7 – #9,each cycle was 40 minutes long and ion energy andbeam current were 3.0 keV and 1.5µA, respectively.Results of the ion profiling studies are summarized inthe Section 4.

3. Theory

Photoelectron spectrum is formed by not scattered,elastically scattered and inelastically multiply scat-tered photoelectrons. Analysis of peaks formed bynot scattered and elastically scattered electrons giveslayer-by-layer chemical and phase composition infor-mation (line-shape analysis). In this case, contribu-tion of inelastically scattered photoelectrons is con-sidered as unwanted background. Consequently, ac-curacy of the analysis depends critically on the pro-cedure of background subtraction. Hence, analysisof multilayer and multicomponent samples is signifi-cantly complicated, as peaks of elastically scatteredelectrons will overlap each other and the peaks of in-elastically scattered electrons.

Identification of layer-by-layer chemical and phasesurface composition includes sequential solving ofthe following three problems: (1) Subtraction ofthe background due to inelastically scattered elec-trons; (2) Decomposition of the spectrum into its con-stituent peaks (extracting of intensity and position ofthe peaks); (3) Extracting of layers thicknesses of themultilayer sample. The first and the second problemsare largely related. Unknown parameters that affectcalculation of both background, and elastically scat-tered photoelectron peaks should be defined jointly.

3.1. Background Subtraction

Background subtraction in XPS analysis, mostcommonly follows methods of Shirley [10] andTougaard [11], which give relatively simple calcula-tion algorithms. Shirley method is purely mathemat-ical technique, which does not account for specificsof electron inelastic scattering in solid. Because ofthat, background subtraction accuracy is often un-predictable. Method of Tougaard is based on the ap-proximate solution for multiple electron scattering insolid [12]. This solution assumes differential inelas-tic scattering cross section of electrons to be depthindependent. Accuracy of background subtraction iscritically dependent on the right choice of the dif-ferential inelastic scattering cross section. Tougaardsuggests two kinds of functions (bi-parametric [13]and tri-parametric [14]) for defining of differential in-elastic scattering cross section. However, even if itgets possible to make right choice of the parameters,which define differential inelastic scattering cross sec-tion in the bulk of solid, the method still suffersfrom missed account for difference between inelas-tic scattering in bulk and at the surface. Paper [15]presents Advanced Tougaard Background Method forsurfaces, which structure can be presented as a se-quence of layers. It is based on representation ofthe measured spectrum as a superposition of eachlayer partial spectrum followed by applying Tougaardmethod to each of them. Problematic though is howto find the partial spectra data. In paper [15], re-cursive procedure is suggested for that. Provided theright first approximation is found right, the algorithmcan demonstrate a reasonable convergence.

3

The following formula that accounts for inelasticscattering both in bulk and at the surface (deriva-tion is presented in Appendix Appendix A) will beused for calculation of the background in the rangeof energies between Emin to Emax:

Background(E ) = A

Emax∫E

j (E′) xSB (E − E′) dE′

(1)where j (E) is the measured flux of photoelectronswith energy E; A is calculated to match backgroundflux at Emin; xSB (∆) is the generalized orthonormal-ized per unity differential inelastic scattering crosssection (further on, orthonormalized per unity differ-ential inelastic scattering cross section will be referredas inelastic indicatrix), ∆ is the energy loss. xSB (∆)depends on surface excitation parameter (SEP ), aswell as on inelastic indicatrices of scattered photoelec-trons in the bulk xB (∆) and at the surface xS (∆)ofthe sample:

xSB (∆) = xB (∆)−∆∫

0

LS (∆− ε)xB (ε) dε+LS (∆) ,

(2)where LS (∆) is calculated following the formula:

LS (∆) ≈N∑n=1

(−1)n+1 SEP

n

n!yn (∆) ,

N is the maximum accountable multiplicity of in-elastic scattering, yn (∆) a the multiple inelas-tic indicatrices, y1 (∆) = xS (∆), yn (∆) =∫∆

0yn−1 (∆− ε) y1 (ε) dε. Parameter SEP depends

on energy of photoelectron, composition and surfacestate. There are different analytic expressions forSEP [16, 17, 18]. Chen [16] proposed a simple ex-pression for the SEP for the surface interaction withan electron with energy E at an angle θ in respect tothe surface normal:

SEP =aCH√E cos θ

(3)

where aCH is the material dependent parameter.

Fig. 1: XPS spectra: line Nb 3d. Circles: experimental data[4], Al anode with a monochromator; criss-crosses: experimen-tal data [4], Mg anode without a monochromator; solid line:calculation by formulae (1) – (8); dashed line: backgroundcalculated by formula (1) – (5)

Electrons in solid loose energy for ionization, ex-perience strong inelastic scattering due to excitationof surface and bulk plasmons, etc. Differential in-elastic scattering cross section can be accounted inthe frame of complex dielectric constant formalism[19, 20]. However, for practical calculations, it ismore convenient to use more simple approximatedforms. Further on, we will use an expression, in whichenergy losses for excitation of plasma oscillations, aswell as losses for ionization of inner electron shells arerepresented:

xin (∆) =σpl

σtotxpl (∆) +

σion

σtotxion (∆) , (4)

where σpl and σion are the full cross sections for en-ergy losses due to plasmon excitation and ionization,σtot = σpl+σion is the full inelastic scattering crosssection. We calculate the orthonormalized differ-ential ionization cross section following the formulafrom paper [21]. For calculations of orthonormal-ized differential cross section for energy loss due toplasmon excitation, we suggest to use formula provedworking well for REELS calculations [22, 23]:

xpl (∆) = Anorm∆α(

∆2 − ε2pl

)2

+ (γ∆)4−β

(5)

4

Fig. 2: Inelastic scattering indicatrices. Solid line: the general-ized inelastic indicatrix xSB (∆) (calculation by formula (2));dash-and-dotted line: the inelastic surface indicatrix xS (∆)multiplied by the SEP for scaling (calculation by formula (5));dashed line: the inelastic volume indicatrix xB (∆) (calcula-tion by formulae (4) and (5))

where εpl is the energy of plasma oscillations, α, βare parameters defining the order of xpl dependenceon energy loss, γ is a parameter, which defines peakwidth, value of Anorm is defined by normalization con-dition

∫∞0xpl (ε) dε = 1. Applying of α = 1, β = 2,

εpl =√C, γ = 2

√C to Eq.(5) reduces it to the

bi-parametric Tougaard function [13]. Applying ofα = 1, β = 2, εpl =

√C, γ =

√D, to Eq.(5) reduces

it to the tri-parametric Tougaard function [14].Figures 1, 2 and 3 show the results of background

calculation for spectrum line Nb3d following the pre-sented approach. Circles (Figs. 1 and 3) and crosses(Fig. 1) present experimental data for pure uniformNb sample taken from Handbook of X-ray Photo-electron Handbook [4]. Circles present experimen-tal data recorded with X-ray source with Al anodeand monochromator, while crosses – with Mg anodeand without monochromator. Dashed line at Fig. 1shows background calculated following Eq. (1). Forcalculations, Eq. (2) for generalized inelastic indi-catrix was applied. Parameters for background andelastic peaks calculations were found jointly throughfitting procedure based on the Marquardt and Leven-berg non-linear least squares curve fitting algorithmof [24]. Upper panel of Fig.1 presents difference be-tween experimental and calculated spectra (Residu-als) proving excellent agreement between experiment

Fig. 3: XPS spectra: line Nb 3d. Circles: experimental data[4], Al anode with a monochromator; solid line (b): calculationby formulae (1) – (8); dashed line (a): background: 1: calcu-lation by the Shirle method, 2 – calculation by the Tougaardmethod, 3 –calculation by formulae (1) – (5)

and calculations (Adjusted R squared R2 = 0.9945,mean relative error 2%). Method for elastically scat-tered photoelectrons peaks calculation along with theparameters for the Nb3d line are communicated inthe section 3.2. Figure 2 shows generalized inelas-tic indicatrix xSB (∆) calculated following formula(2) with SEP = 0.24 (solid line); inelastic surfacescattering indicatrix xS (∆) multiplied by SEP , cal-culated following formula (5) with the following pa-rameters αS = 1.10, βS = 2.08, εpl S = 10.4 eV,γS = 5.5 (dash-dotted line); inelastic bulk scatter-ing indicatrix xB (∆) calculated following the for-mulas (4) and (5) with the following parametersαB = 1.10, βB = 2.08,εpl B = 20.5 eV, γB = 10.5 ion-isation thresholds in Grysinsky formula J1 = 37.4 eV,J2 = 39.2 eV (dashed line). The highest error of thebackground calculations appears to be for ionizationlosses. That is due to Grysinsky formula is an ap-proximation. Figure 3 shows comparison of exper-imental data for the Nb3d line (marked with b atthe plots) and that calculated by different methods(marked with a at the plots): 1 – Shirley method, 2 –Tougaard method, tri-parametric formula (C = 425,D = 88), 3 - the presented method, Eqs. (1) – (5).Parameters used for calculation by each method weredifferent and optimized for minimum dispersion fol-lowing the Marquardt and Levenberg algorithm. It isseen that the presented method gives the best results.

5

3.2. Line Decomposition

Structure of XPS peaks may be quite complex dueto spin-orbit interaction, chemical shift and presenceof satellite peaks. Additionally, shape and width ofthe peaks themselves depend on various factors, andthe peaks can overlap each other. For example, Nb3dline may contain up to six doublets (total 12 peaks),as Nb forms 5 different oxides (maximum oxidationstate for niobium J = 5). Accurate decomposition ofso complex lines calls for careful account for variousfactors defining peaks shape and intensity.

Shape of spectral line LS (E) of photoelectronswith kinetic energy E is determined by convolu-tion of functions describing natural shape of theline and its instrumental broadening. Natural shapeof the line is defined by Doniach-Sunjic equation[25] D (E, δ, aDS), where δ is natural width of elec-tron level, aDS is the Anderson singularity index[26]; if aDS = 0, the Doniach-Sunjic equation re-duces to Lorentz function. Instrumental broaden-ing follows Gaussian function G (E,W ), where W =√W 2sp +W 2

hν , Whν and Wsp are X-ray radiation and

instrumental broading linewidths.

LS (E) =

∫D (E′, δ, aDS)G (E − E′,W ) dE′, (6)

We account for nonmonochromaticity of X-ray sourceradiation through the following expression:

LS1 (E) = LS (E) +

K∑k=1

Isat k LS (E + ∆Esat k) ,

(7)where Isat and ∆Esat are relative intensities and en-ergy shifts of satellites. These parameters depend onmaterial of X-ray source anode. We use the values ofthese parameters communicated in [4].

Spectra of photoelectrons of p- , d-... shells havedoublet structure due to spin-orbital interaction.Shape of the spin-orbital doublets is described by thefollowing expression:

LS2 (E) =1

1 + αLS1 (E) +

α

1 + αLS1 (E −∆ESO) ,

(8)

where α is the ratio for intensities of spin-orbital split-ted lines (α = 1/2 for p-shell, and α = 2/3 for d-shell), ∆ESO is the spin-orbital interaction energy.

Line under analysis can consist of doublet of freeelement, either of doublets of elements in differentchemically bonded states. In the latter case, complexline shape is described by expression:

LSΣ (E) = I0 LS2 (E) +

J∑j=1

Ij LS2 (E −∆ECS j) .

(9)where ∆ECS j is the chemical shift energy, Ij is thedoublet line intensity, J is the number of the doubletlines.

For accurate decomposition of the complex line de-pends on the values of the parameters δ and aDS andenergies ∆ESO and ∆ECS . Once those are defined,number of variable parameters gets minimal and in-tensities of the doublet lines can be found by fittingalgorithms, e.g. Levenberg-Marquardt.

The natural line width δ is defined by the lifetimeτ of ionized state formed after photoemission. Asa consequence of Heisenberg’s uncertainty principle,δ ∼ ~/τ . The hole lifetime is defined by radiativerecombination process emitting characteristic radi-ation, or Auger recombination emitting an Auger-electron. Lifetime of vacancy depends on the numberof valence electrons Nv [27]. Auger-recombinationand photo-fluorescence can be resolved within thesame electron shell. Because of that, natural linewidth may be different for the peaks in a doublet.We propose to approximate δ with expression:

δ = αsoδ0

(ωf

(Nv

Nv 0

)af+ ωO

(Nv

Nv 0

)aO)(10)

where δ0 is the natural line width for free (no chemi-cally bonded) element, Nv 0 is the number of valenceelectrons for free element, αso is the coefficient ac-counting for line broadening due to spin-orbital split-ting (αso = 1 for the main peak in a doublet), ωf isthe fluorescence yield, ωO = 1− ωf is the Auger de-cay yield. Dependence of fluorescence yield on atomicnumber is presented in paper [28]. Coefficients afand aO can be found from analysis of experimen-

6

Fig. 4: Dependence of the natural width of the photoelectronoxide line on the atomic number. Circles: experiment [29],criss-crosses: calculation by formula (10)

tal data for natural line widths and calculations fol-lowing formula (10). Figure 4 presents experimentaldata (circles) for natural line widths of oxides de-pendence on atomic number Z of elements [29] alongwith calculations (crosses) by formula (10) with pa-rameters giving the best approximation (af = 0.4305,aO = 0.5993 for transition metals, and af = 0.9444,aO = 0.5627 for all others). Mean relative errorachieved was 6%.

For pure elements, we suggest taking their naturalwidth δ0, binding energy BE0 and spin-orbit interac-tion energy ∆ESO from experimental data of Hand-book of X-Ray Photoelectron Spectroscopy [4]. Fur-ther on, those parameters are kept fixed. For mostaccurate defining of line parameters for element, wesuggest using two sets of of experimental data: spec-tra recorded with an X-ray source with Al anode andmonochromator, along with those with Mg anode andwithout monchromator. Background is suggested tosubtract following the approach presented in Section3.1. Figure 1 presents results calculated with thefollowing Nb3d line parameters: δ0 = 0.0693 eV,αso = 2.30, αDS = 0.136, BE0 = 202.40 eV,∆ESO =2.72 eV. Coefficients αso and αDS depend on com-position and condition at the surface and are fittingparameters for each sample.

For chemically bonded elements, we suggest cal-culating the natural line width δ0 following Eq.(10).Chemical shift energy practically is linearly propor-

tional to the oxidation state. For that, it is sufficientto find the chemical shift energy for the highest oxi-dation state of the element. For example, for niobiumoxide, we used ∆ECS Nb2O5

= 5.31 eV [30]. Section4 communicates calculation results for the lines fol-lowing the above presented approach.

3.3. Extracting of thicknesses of layers

In paper [31], the formula for calculation of ox-ide layer thickness is derived for the bi-layer model.In reality however surface always has more complexstructure and hence has to be presented as multilayer.In paper [2] , systems of nonlinear equations are pre-sented, which solution gives thicknesses of surfacelayers. When the number of the layers is large, suchcalculation scheme starts behaving unstable. In thepaper, based on the approach described in [5, 32, 31],the simple formula for extracting of the layers thick-nesses is proposed (derivation of that is presented inthe Appendix Appendix B):

di = λi cos θ ln

(Ii/ (ni ωp→e i (γ)λi)∑i−1j=0 Ij/ (nj ωp→e j (γ)λj)

+ 1

),

(11)where di is the thickness of i-th layer, n is the atomicconcentration, ωp→e (γ) is the differential cross sec-tion of photoelectron production [33], γ is the an-gle between the incident radiation and direction toenergy analyzer, λ is the inelastic mean free pathlength (IMFP) calculated following TPP2M formula[34], θ is the angle between direction to energy ana-lyzer and surface normal, Ii is the intensity of thei-th peak. Layer numbering increases from the sub-strate and up, so that number 0 corresponds to thesubstrate. In case of bi-layer, Eq. (11) reduces to theformula presented in [31].

To consider elastic scattering effects, IMFP in eq.(11) is to be replaced by the corresponding EAL(Effective-Attenuation-Length):

di = Li cos θ ln

(Ii/ (ni ωp→e i (γ)Li)∑i−1j=0 Ij/ (nj ωp→e j (γ)Lj)

+ 1

),

(12)

7

where L is the average EAL for photoelectrons scat-tered by the substrate and the film that travel inthe film. Values of L can be estimated from a NISTdatabase [35]. We use expression derived in work [36]

L = λ

(1− 0.735

λ

λ+ λtr

), (13)

and λtr = 1nσtr

is the transport mean free path(TMFP), σtr is the transport cross section of an el-emental solid. Values of transport cross sections areavailable from the NIST Electron Elastic-ScatteringCross-Section database [37].

For calculating of layer thicknesses in a multilayersample, assume first that the sample is semi-infinite,metallic and uniform. If oxidation occurred by ex-posure to oxygen containing gas mixture outside theanalysis chamber, then the oxidation states of thesurface will decrease from the surface towards inte-rior of the sample [5]. Also, one can expect pres-ence of some hydrocarbons at the very surface, e.g.residuals from the protecting polymer layer (see Ex-perimental section). Calculation of layer thicknesswill follow a number of consequent steps. First, letassume surface consisting of a number of uniform lay-ers, inside each of which oxidation state is constant.Oxidation state can be not-integer. If in course ofcalculations thickness of certain layer is found be lessthan one monolayer (ca. 0.5 nm), that is combinedwith the neighboring one, which further on is consid-ered uniform and multicomponent. Contribution ofeach layer component is accounted as its relative con-centration in the layer. Calculation results for multi-layer multicomponent sample is presented in Table 2of Section 4.

4. Results and Discussion

In this work, multilayer niobium suboxide filmswere studied. After loading the sample into the an-alytic chamber and after each sputtering cycle, XPSsurvey and detailed spectra of the lines O1s, C1s,Nb3p and Nb3d were recorded. Figure 5a shows thesurvey spectra. Number 0 marks spectra before sput-tering, numbers 1, 3 and 8 mark spectra after corre-sponding number of the sputtering cycles. Standard

XPS analysis of the sample before sputtering iden-tified presence of Nb, O and C, Fig. 5a. Relativeconcentrations of those before sputtering were foundto be cNb = 14%, cO = 53% and cC = 33%. Af-ter the first cycle of sputtering, peaks at the carbonline C1s vanished. Relative concentration of Nb aftereach sputtering cycle was as following: 1 – 47%, 2 –73%, 3 – 82%, 4 – 82%, 5 – 83%, 6 – 84%, 7 – 93%,8 – 96%, 9 – 98%. Abrupt increase of Nb relativeconcentration after the cycle 7 is due to the changeof sputtering cycle parameters (see Section 2).

Standard XPS analysis calculates relative concen-trations assuming the sample is uniform at the wholeinformation depth of analysis. However, both be-fore and after sputtering, the sample is nonuniform,multicomponent and multilayer. For quantitativedepth profile analysis, recorded lines needs to de-composed into the partial peaks formed by photoelec-trons emitted by the different chemically bonded ele-ments. Figs. 5b, 5c and 5d demonstrate experimentalspectra and their interpretation following the methodpresented in the Section 3. Circles show recorded de-tailed spectra, the solid lines show calculated spec-tra. Background removal followed the method pre-sented in the Section 3. For all calculated peak spec-tra, the instrumental broadening Wsp = 0.575 eVwas used, as all the detailed spectra were recordedwith the same parameters for energy analyser oper-ated in FAT mode with the pass energy of 20 eV.The surface state changed after each sputtering cycle,consequently, so did background parameters. TheDoniach-Sunjic asymmetry coefficient αDS dependson composition and state of surface and thus werethe same for each spectral line. This allowed findingthe αDS values for spectra after each sputtering cycle.Linewidths δ for each peak were calculated followingEq. (10). Details of the spectra before and after cy-cles 1,3 and 8 of sputtering are summarized in Table1. In Table 1a, the key global, i.e. the common forall spectral peaks, parameters are presented: general-ized indicatrix parameters (εpl B and εpl S are the en-ergies of bulk and surface plasmons), aCH parameterfor SEP calculation following formula (3) as well asαDS coefficient. Table 1b shows, into which peaks thelines are decomposed: binding energy BE, chemical

8

(a) (b)

(c) (d)

Fig. 5: XPS spectra. Circles: experimental data, Mg anode without a monochromator; solid line: calculation by formula (1) –(8). The number show sputtering cycles. (a) Target: survey spectra; (b) target: line O 1s; (c) target: line C 1s; (d) target: lineNb 3d

(a) (b)

Fig. 6: XPS spectra. Circles: experimental data, Mg anode without a monochromator; solid line: calculation by formulae (1) –(8); dashed line (a): background: calculation by formulae (1) – (5); dashed-and-dotted line: separate calculated peaks. (a)Target: line Nb 3d; (b) target: line Nb 3p

9

Table 1: Global and local parameters of line decomposition

(a)

0 1 3 8εpl B ,eV

εpl S ,eV

aCH αDSεpl B ,eV

εpl S ,eV

aCH αDSεpl B ,eV

εpl S ,eV

aCH αDSεpl B ,eV

εpl S ,eV

aCH αDS

24.6 14.7 19.8 0.028 26.8 13.8 23.7 0.093 20.9 10.7 10.0 0.123 20.5 10.4 7.8 0.133

(b)

0 1 3 8BE,eV

c,%

Iσpλ

FormulaBE,eV

c,%

Iσpλ

FormulaBE,eV

c,%

Iσpλ

FormulaBE,eV

c,%

Iσpλ

Formula

O 1s530.8 73 16.32 NbOx 530.8 89 14.33 NbOx 530.8 100 4.67 NbOx 530.8 100 1.18 NbOx

531.8 16 3.66 −C = O 531.4 11 1.69 Nb(HO)x533.1 11 2.44 −C−O

C 1s284.6 64 8.76 CHx

285.7 21 2.93 −C−O286.6 15 2.05 −C = O

Nb 3d202.4 6 0.53 Nb 202.4 15 2.46 Nb 202.4 77 19.62 Nb 202.4 91 22.90 Nb203.4 1 0.07 Nb2O 203.4 10 1.33 Nb2O 203.4 15 3.94 Nb2O 203.4 9 2.38 Nb2O207.7 93 6.55 Nb2O5 204.4 30 4.10 NbO 204.4 3 0.77 NbO

205.2 10 1.44 Nb(HO)x 205.5 3 0.64 Nb2O3

205.5 12 1.74 Nb2O3 206.5 2 0.36 NbO2

206.5 14 1.95 NbO2

207.7 9 1.26 Nb2O5

Table 2: Layer thicknesses based on the XPS results

0 1 3 8

Layerd,

nmFormula Layer

d,nm

Formula Layerd,

nmFormula Layer

d,nm

Formula∑12.0

∑6.2

∑0.8

∑0.6

3 1.40.36Cx(HO)y+

0.64CHx4 0.5

0.31Nb(HO)x+0.27Nb2O5+0.42NbO2

1 0.8

0.07NbO2+0.13Nb2O3+0.13NbO+0.67Nb2O

1 0.6 Nb2O

1 9.6 Nb2O5 3 1.2 Nb2O3 Substr. Nb Substr. Nb2 1.0 Nb2O 2 1.7 NbOSubstr. Nb 1 2.8 Nb2O

Substr. Nb

10

formulas, relative concentration c, value na = Iσpλ

,

where I is the intensity of a single or doublet peak,σp is the photoionization cross section for the partic-ular line, λ is the IMFP calculated for a particularcompound/chemical formula. Parameter na is pro-portional to the atomic concentration n of particularelement. Calculated for the different lines, but forthe same compound chemical formula, na should beproportional to its stoichiometric coefficients.

For the highest decomposition accuracy, both linesNb3d and Nb3p. were analysed. For demonstrationof the analysis flow, let follow step by step analysisof the most complicated case, surface after the firstsputtering cycle. Figure 6 presents detailed spectra ofthe Nb3d line (Fig. 6a) and Nb3p (Fig. 6b) after thefirst cycle of sputtering. Dots present the recordeddata, solid line is for the calculated spectrum, dashedline shows the background calculated followed themethod presented in the Section 3.1, dash-dotted lineis for partial doublet peaks. The same backgroundand partial peak parameters (Tabl. 1) were used forcalculation of both Nb3d and Nb3p lines.

Parameter na helps assessing how adequate is de-composition of a spectral line. Let consider a layercontaining a number of metal oxides MOxj (xj = j/2,where j is metal oxidation degree in oxide). Each ox-ide has a relative concentration cj . Then, a meanfor the layer stoichiometric coefficient for oxygen is〈x〉c =

∑j cj

j2 . Suppose, analysis of an XPS line

of the metal gave the partial parameters nMaj , while

analysis of line O1s gave nOa . Then mean stoichio-

metric coefficient for oxygen is 〈x〉n =nOa∑j n

Ma j

, as the

na parameter is proportional to the atomic concen-tration. Naturally, two ways for stoichiometric co-efficient calculation should give the same result. Inthe other words, that is the criterion for the detailedspectra decomposition into the partial peaks. Thefollowing condition should be satisfied:

∑j

cj xj =nOa∑j n

Maj

. (14)

It is worth mentioning that the above criterion (14)is satisfied for the presented decomposition into par-tial peaks (Fig. 5 and Tabl. 1). For example, for the

most complicated case of the spectra recorded afterfirst sputtering cycle, the mean stoichiometric coeffi-cient of oxygen, when calculated through the relative

concentrations, 〈x〉c =10· 12 +30· 22 +12· 32 +14· 42 +9· 52

10+30+12+14+9 =1.3800, while when calculated through the na param-eter, 〈x〉n = 14.33

1.33+4.1+1.74+1.95+1.26 = 1.3805.Decomposition of the detailed spectra into the par-

tial peaks following the approach presented in theSection 3.3 allowed extracting thicknesses of oxideand suboxide layers of niobium. Layer thicknesseswere calculated by Eq. (12). Table 2 summarizes theresults for chemical and phase depth profile analysisof the surface before and after 1, 3 and 8 sputteringcycles.

The probing information depth calculated by theformula (12) for the bilayer model (I1/I0 = 100/1) is15 nm.

5. Conclusions

In this paper, the new method for XPS chemicaland phase depth profile analysis has been presented.The method is based on the most accurate solutionof the XPS key problems (see Section 3). It is worthmentioning that the XPS depth profile analysis is areverse problem with multiple unknown parameters.For the correct solving of the problem, we propose:joint solving of the key problems using the global pa-rameters for all detailed spectra; accounting for dif-ferent lines of an element for their joint decomposi-tion into partial peaks; decomposition quality assess-ing with a help of suggested criterion.

Appendix A. Background

A photoelectron born at a depth z with energy E0

needs to travel the length u in the sample’s matterbefore exiting the sample surface at the angle θ tothe surface normal being registered with an energy Eby an energy analyzer. On the way, it looses energy∆ = E0−E. Flux density of such electrons is definedby the relation [38, 39]:

q (z,∆, θ0, θ) = nωp→e (γ)Tin

(∆,

z

cos θ

)(A.1)

11

where n is the atomic concentration, ωp→e is thedifferential photoelectron creation cross section, γ isthe angle between the direction of photon incidenceand travel direction of the created photoelectron;λ = 1

nσinIMFP, σin is the inelastic scattering cross

section; θ0 is the angle between the surface normaland direction of photon incidence; Tin (∆, u) is thelayer’s inelastic transmission function, ∆ is the elec-tron energy loss, u is the photoelectron length oftravel. For the transmission function, let follow thegeneral solution after Landau [40]:

Tin (∆, u) =1

2πi

+i∞∫−i∞

e−un (σin−W (p))ep∆dp,

where W (p) is the Laplace image of differential in-elastic scattering cross section ωin (∆). In Laplacespace, transmission function has a simple form:

Tin (p, u) = exp(−uλ

(1−X (p))),

where X (p) = W (p)σin

is the Laplace image of inelas-

tic indicatrix xin (∆) = ωin(∆)σin

, which is the or-thonormalized differential inelastic scattering crosssection. Flux density of all the photoelectrons exitingthe sample Q (∆) is defined in the Laplace space asfollowing:

Q (p) =

∞∫0

nωp→e (γ) e−z

λ cos θ (1−X(p))dz =

nωp→e (γ)λ cos θ

1−X (p).

(A.2)

Let introduce function Q (p) = Q(p)nωp→e(γ)λ cos θ ,

then from (A.2) follows:

Q (p)− Q (p)X (p) = 1. (A.3)

Coming back to the natural space and using theproperty of Laplace transformation, we get the fol-

lowing equation:

δ (∆) = Q (∆)−∆∫

0

Q (ε)xin (∆− ε) dε. (A.4)

The peak of not scattered and elastically scatteredphotoelectrons corresponds to the Dirac delta func-tion δ (∆). The convolution integral defines back-ground due to inelastic multiple scattered photo-electrons. Q (E) function is proportional to mea-sured photoelectron flux j (E). Consequently, theTougaard formula for background [12] can be ob-tained:

Background(E ) = A

Emax∫E

j (E′) xin (E − E′) dE′,

(A.5)where A is defined by the spectrum point at the en-ergy Emin.

Formula (A.5) is obtained with the assumption ofthe sample uniformity across the sample depth. How-ever, for inelastic scattering real sample is alwaysnonuniform. Electron energy losses at the samplesurface and in the bulk follow different relations. Asthe first approximation, in a semi-infinite sample weselect very thin plane-parallel surface layer with thethickness dS , where energy losses are defined by sur-face plasmon excitation. Outside the selected layer,the energy losses are defined by the bulk plasmonexcitation and ionization losses. This way, losses inthis layer are described by inelastic indicatrix xS (∆)(Laplace image XS (p)), while outside the layer byxB (∆) (Laplace image XB (p)). The IMFP in thislayer is designated as λS , outside the layer λB . Then,the Laplace image of transmission function for thephotoelectrons passing a layer belonging to the bulkof the sample with thickness z and a thin layer withthickness dS at the angle θ to the surface normal isdefined as:

Tin (p, u) = e− zλB cos θ (1−XB(p))

e− dSλS cos θ (1−XS(p))

.(A.6)

12

Surface excitation parameter (SEP ) can be repre-sented as:

SEP =dS

λS cos θ. (A.7)

IMFP of photoelectrons is proportional to their en-ergy, λ ∼ Ea. Parameter a is usually within therange of 0.5...0.9. With a = 0.5 (A.7) gets reduced tothe Chen formula [16]. Plugging (A.6) to (A.1) andintegrating across the whole sample thickness and ac-counting for (A.7) Laplace image of the full flux den-sity of all photoelectrons escaping the sample surface:

QSB (p) =nωp→e (γ)λB cos θ

1−XB (p)e−SEP (1−XS(p)).

(A.8)Introducing the functions:

XSB (p) = 1− e−SEP XS(p) (1−XB (p)) , (A.9)

˜QSB (p) =QSB (p)

nωp→e (γ)λB cos θ e−SEP

a relation similar to (A.3) is obtained:

QSB (p)− QSB (p)XSB (p) = 1. (A.10)

Similarly as for deriving (A.5), the background calcu-lation formula accounting for inelastic scattering atthe surface and in bulk is obtained:

Background(E ) = A

Emax∫E

j (E′) xSB (E − E′) dE′.

(A.11)Fundamental difference between Eqs. (A.5) and

(A.11) though is that the function under integralxSB (∆) in (A.11) depends on SEP , as well as inelas-tic photoelectron scattering indicatrix in bulk xB (∆)and at the surface xS (∆). For deriving of the calcu-lation formula for xSB (∆), let re-write Eq. (A.9) inthe following form:

XSB (p) = XB (p)−XB (p)L (p) + L (p) ,

where L (p) = 1 − e−SEP XS(p). L (p) func-tion can be expanded in a power series

L (p) =∑∞n=1 (−1)

n+1 SEPn

n!XnS (p). After re-

versed Laplace transformation the obtained formulafor xSB (∆) are the following:

xSB (∆) = xB (∆)−∆∫

0

LS (∆− ε)xB (ε) dε+LS (∆)

(A.12)

where LS (∆) ≈∑Nn=1 (−1)

n SEPn

n!yn (∆),

y1 (∆) = xS (∆), yn (∆) =∫∆

0yn−1 (∆− ε) y1 (ε) dε,

N is the maximum accountable multiplicity ofinelastic scattering.

Appendix B. Layer Thickness

The method for calculation of the layers thick-nesses in multilayer model is based on the approachpresented in the papers [5, 32, 31]. The flux of pho-toelectrons born at the depth z with the energy E0

loselessly escaping the sample surface at the angle θto its normal is defined by the following formula:

q (z, θ0, θ) = nωp→e (γ) exp(− z

λ cos θ

)(B.1)

where n is the atomic concentration, ωp→e is thedifferential electron creation cross section, λ is thephotoelectron’s IMFP, γ is the scattering angle. Fordefining of flux density of the photoelectrons escap-ing a uniform layer with a depth di, integrating ofEq. (B.1) across the whole layer thickness is needed:

Q (di, θ0, θ) =

di∫0

q (z, θ0, θ) dz. (B.2)

After integration, we obtain:

Q (di, θ0, θ) = ni ωp→e i (γ)λi cos θ(

1− e−di

λi cos θ

).

(B.3)

13

Designating Ti = exp(− diλi cos θ

), Q∞i =

Qi (∞, θ0, θ) = ni ωp→e i (γ)λi cos θ allows rewritingEq. (B.3) in a compact form:

Qi = Q∞i (1− Ti) .

is proportional to the measured peak intensity Ii. Leta sample consist of N layers over a substrate witheach i-th layer having di thickness. Numbering of thelayers does from the substrate and up (the substrategets number 0). The flux density of photoelectronsborn within the i-th layer and passed the layers withnumbers from i+ 1 to N is the following:

Qi,...,N = Q∞i (1− Ti)Ti+1 · . . . · TN .

For all layers and the substrate, the following sys-tem of non-linear equations is obtained:

Q0,...,N = Q∞0 T1 · . . . · TNQ1,...,N = Q∞1 (1− T1)T2 · . . . · TN· · ·Qi,...,N = Q∞i (1− Ti)Ti+1 · . . . · TN· · ·QN = Q∞N (1− TN )

From the system, thicknesses di of the layers can befound. For that let us divide the flux density Qi,...,Nof photoelectrons generated in the layer i to the fluxdensity Q0,...,N of photoelectrons generated in thesubstrate. This relation will be equal to the relationof the corresponding peak intensities

IiI0

=Q∞iQ∞0

(1− Ti)T1 · . . . · Ti

. (B.4)

Let us introduce fi = IiQ∞0 / (Q∞i I0). Then expres-

sion (B.4) transforms into an iterative formula

1

Ti= fi · T1 · . . . · Ti−1 + 1,

from that an expression for Ti

1

Ti=

fifi−1 + . . .+ f1 + 1

+ 1.

may be derived. Next, using the introduced designa-tions and functions, we get a simple formula for layerthicknesses

di = λi cos θ ln

(Ii/ (ni ωp→e i (γ)λi)∑i−1j=0 Ij/ (nj ωp→e j (γ)λj)

+ 1

).

(B.5)

References

[1] C. Powell, New data resources and applicationsfor aes and xps, Journal of Surface Analysis20 (3) (2014) 155–160.

[2] C. Olsson, D. Landolt, Atmospheric oxidationof a Nb-Zr alloy studied with XPS, CorrosionScience 46 (1) (2004) 213–224. doi:10.1016/

S0010-938X(03)00139-2.

[3] A. Trifonov, A. Lubenchenko, V. Polkin,A. Pavolotsky, S. Ketov, D. Louzguine-Luzgin,Difference in charge transport properties of ni-nbthin films with native and artificial oxide, Jour-nal of Applied Physics 117 (12) (2015) 125704.

[4] J. Chastain, R. C. King, J. Moulder, Handbookof X-ray photoelectron spectroscopy: a referencebook of standard spectra for identification andinterpretation of XPS data, Physical ElectronicsEden Prairie, MN, 1995.

[5] M. Grundner, J. Halbritter, Xps and aes studieson oxide growth and oxide coatings on niobium,Journal of Applied Physics 51 (1) (1980) 397–405.

[6] A. Darlinski, On angle resolved x-ray photoelec-tron spectroscopy of oxides, serrations, and pro-tusions at interfaces, Journal of Vacuum Science& Technology A: Vacuum, Surfaces, and Films5 (4) (1987) 1235. doi:10.1116/1.574779.

[7] J. Halbritter, On the Oxidation and on theSuperconductivity of Niobium, Applied PhysicsA 43 (1987) (1987) 1–28. doi:10.1007/

BF00615201.

14

[8] M. Kuznetsov, A. Razinkin, A. Ivanovskii, Ox-ide nanostructures on a nb surface and relatedsystems: experiments and ab initio calculations,Physics-Uspekhi 53 (10) (2010) 995.

[9] Z. Weibin, W. Weidong, W. Xueming, C. Xinlu,Y. Dawei, S. Changle, P. Liping, W. Yuying,B. Li, The investigation of nbo2 and nb2o5 elec-tronic structure by xps, ups and first principlesmethods, Surface and Interface Analysis 45 (8)(2013) 1206–1210.

[10] D. A. Shirley, High-resolution x-ray photoemis-sion spectrum of the valence bands of gold, Phys-ical Review B 5 (12) (1972) 4709.

[11] S. Tougaard, Practical algorithm for backgroundsubtraction, Surface Science Letters 216 (3)(1989) A330. doi:10.1016/0167-2584(89)

91270-X.

[12] S. Tougaard, I. Chorkendorff, Differential inelas-tic electron scattering cross sections from exper-imental reflection electron-energy-loss spectra:Application to background removal in electronspectroscopy, Physical Review B 35 (13) (1987)6570–6577. doi:10.1103/PhysRevB.35.6570.

[13] S. Tougaard, Low energy inelastic electron scat-tering properties of noble and transition metals,Solid State Communications 61 (9) (1987) 547–549. doi:10.1016/0038-1098(87)90166-9.

[14] S. Tougaard, Universality Classes ofInelastic Electron Scattering Cross-sections, Surface and Interface Analy-sis 25 (November 1996) (1997) 137–154.doi:10.1002/(SICI)1096-9918(199703)25:

3<137::AID-SIA230>3.0.CO;2-L.

[15] R. Hesse, M. Weiß, R. Szargan, P. Streubel,R. Denecke, Improved peak-fit procedure forXPS measurements of inhomogeneous samples- Development of the advanced Tougaard back-ground method, Journal of Electron Spec-troscopy and Related Phenomena 205 (2015) 29–51. doi:10.1016/j.elspec.2015.06.013.URL http://dx.doi.org/10.1016/j.elspec.

2015.06.013

[16] Y. Chen, Surface effects on angular distribu-tions in X-ray-photoelectron spectroscopy, Sur-face Science 519 (1-2) (2002) 115–124. doi:

10.1016/S0039-6028(02)02206-9.

[17] K. Salma, Z. Ding, H. Li, Z. Zhang, Surfaceexcitation probabilities in surface electron spec-troscopies, Surface science 600 (7) (2006) 1526–1539.

[18] W. S. Werner, L. Kover, S. Egri, J. Toth,D. Varga, Measurement of the surface excitationprobability of medium energy electrons reflectedfrom si, ni, ge and ag surfaces, Surface science585 (1) (2005) 85–94.

[19] J. Lindhard, On the properties of a gas ofcharged particles mat. fys. medd, K. Dan. Vid.Sel 28 (8).

[20] R. Ritchie, A. Howie, Electron excitation andthe optical potential in electron microscopy,Philosophical Magazine 36 (2) (1977) 463–481.

[21] M. Gryzinski, Classical theory of atomic colli-sions. i. theory of inelastic collisions, PhysicalReview 138 (2A) (1965) A336.

[22] V. Afanas’ev, A. Lubenchenko, M. Gubkin,Quantitative interpretation of eels and reelsspectra, The European Physical Journal B-Condensed Matter and Complex Systems 37 (1)(2004) 117–125.

[23] V. Afanasyev, D. Efremenko, A. Lubenchenko,M. Vos, M. Went, Extraction of cross-sectionsof inelastic scattering from energy spectra of re-flected atomic particles, Bulletin of the RussianAcademy of Sciences: Physics 74 (2) (2010) 170–174.

[24] J. J. More, The levenberg-marquardt algorithm:implementation and theory, in: Numerical anal-ysis, Springer, 1978, pp. 105–116.

[25] S. Doniach, M. Sunjic, Many-electron singular-ity in x-ray photoemission and x-ray line spectrafrom metals, Journal of Physics C: Solid StatePhysics 3 (2) (1970) 285.

15

[26] P. Anderson, Infrared catastrophe in fermi gaseswith local scattering potentials, Physical ReviewLetters 18 (24) (1967) 1049.

[27] D. Spanjaard, C. Guillot, M.-C. Desjonqueres,G. Treglia, J. Lecante, Surface core level spec-troscopy of transition metals: A new tool for thedetermination of their surface structure, SurfaceScience Reports 5 (1) (1985) 1–85.

[28] M. Chen, H. Crasemann, B.and Mark, Relativis-tic m-shell radiationless transitions, Physical Re-view A 21 (2) (1980) 449.

[29] J. Shea, Handbook of monochromatic XPS spec-tra - The elements and native oxides [BookReview], IEEE Electrical Insulation Magazine19 (4). doi:10.1109/MEI.2003.1226740.

[30] A. V. Naumkin, A. Kraut-Vass, C. Pow-ell, NIST X-ray photoelectron spectroscopydatabase, Measurement Services Division of theNational Institute of Standards and Technology(NIST) Technology Services, 2008.

[31] B. Strohmeier, An esca method for determiningthe oxide thickness on aluminum alloys, Surfaceand Interface Analysis 15 (1) (1990) 51–56.

[32] T. Carlson, Basic assumptions and recent devel-opments in quantitative xps, Surface and Inter-face Analysis 4 (4) (1982) 125–134.

[33] J. Yeh, I. Lindau, Atomic subshell photoioniza-tion cross sections and asymmetry parameters:1¡ z¡ 103, Atomic data and nuclear data tables32 (1) (1985) 1–155.

[34] S. Tanuma, C. Powell, D. Penn, Calculations ofelectron inelastic mean free paths. v. data for 14organic compounds over the 50–2000 ev range,Surface and Interface Analysis 21 (3) (1994)165–176.

[35] C. J. Powell, A. Jablonski, NIST ElectronEffective-Attenuation-Length Database, Version1.3, U.S. Department of Commerce/NIST:Gaithersburg, MD, 2011.URL https://www.nist.gov/srd/

nist-standard-reference-database-82

[36] A. Jablonski, C. Powell, Practical expressionsfor the mean escape depth, the informationdepth, and the effective attenuation length inauger-electron spectroscopy and x-ray photo-electron spectroscopy, Journal of Vacuum Sci-ence & Technology A 27 (2) (2009) 253–261.

[37] A. Jablonski, F. Salvat, C. Powell, NISTElectron-Scattering Cross-Section Database,Version 3.2, U.S. Department of Com-merce/NIST: Gaithersburg, MD, 2010.URL https://www.nist.gov/srd/

database-64

[38] S. Tougaard, P. Sigmund, Influence of elastic andinelastic scattering on energy spectra of elec-trons emitted from solids, Physical Review B25 (7) (1982) 4452.

[39] S. Tougaard, Energy loss in xps: Fundamen-tal processes and applications for quantification,non-destructive depth profiling and 3d imaging,Journal of Electron Spectroscopy and RelatedPhenomena 178 (2010) 128–153.

[40] L. Landau, On the energy loss of fast particlesby ionization, Originally published in J. Phys 8(1944) 201.

16

Recommended